Improvement of optical and electrical properties of ITO thin
, Fulya Turkoglua,b
, Metin Kurta
, Mutlu D. Yamana,c
Fatime G. Akcaa
, Gulnur Ayguna
aDepartment of Physics, Izmir Institute of Technology, 35430, Urla, Izmir, Turkey
bDepartment of Material Science and Engineering, Izmir Institute of Technology, 35430, Urla, Izmir, Turkey cTeknoma Technological Materials Ltd, IZTEKGEB, IZTECH Campus, Urla, Izmir, Turkey
a r t i c l e i n f o
Received 1 December 2014 Received in revised form 26 May 2015
Accepted 16 June 2015 Available online 23 June 2015
Keywords: ITO thinﬁlm Electro-annealing
Large area magnetron sputtering
a b s t r a c t
The effect of electro-annealing in vacuum and air on the optical and electrical properties of ITO thinﬁlms grown by large area DC magnetron sputtering was investigated. Moreover, the performances of the electro-annealed ITO thinﬁlms in vacuum and air were compared. Electro-annealing was performed by applying 0.75, 1.00, 1.25 and 1.50 A constant ac current to the ITO thinﬁlms. It was observed that the crystallinity of theﬁlms was better for the ITO thin ﬁlms electro-annealed in vacuum. The changes in sheet resistance of electro-annealed ITO thinﬁlms with applied currents were detailed. The trans-mittance of theﬁlms increased for both electro-annealing in vacuum and air. A correlation between band-gap and resistivity for all of the electro-annealed thinﬁlms was observed.
© 2015 Elsevier Ltd. All rights reserved.
Transparent conducting oxides (TCOs) have a wide range of applications including transparent electrodes in LCDs, organic light emitting diodes, solar cells, plasma display panels (PDP), trans-parent heat reﬂecting windows as well as surface heaters for cameras, lenses, mirrors, car windows, gas sensors and ohmic contacts for surface-emitting diodes[1e3]. Indium tin oxide (ITO) thinﬁlm is one of the most commonly used materials among the TCO thinﬁlms due to its relatively low resistivity and high optical transmittance in the visible region of the electromagnetic spectrum .
Growth conditions such as oxygen partial pressure, substrate temperature and bias voltage are strongly important parameters for the high electrical conductivity and the transmittance in the visible spectral range of ITO ﬁlms. Several deposition techniques such as thermal evaporation , chemical vapor deposition, electron beam evaporation, solegel, spray pyrolysis, pulsed laser depositionand magnetron sputteringhave been used for years in order to prepare high quality ITOﬁlms. The magnetron
sputtering method is the commonly preferred technique due to the reproducible deposition of theﬁlms.
Annealing of ITO thinﬁlms produced by magnetron sputtering is done to achieve the desired structure and properties of theﬁlms for practical applications . The most common method for the annealing of transparent conductive oxides is thermal annealing . As an alternative, recent studies have reported that the per-formance of deposited ITO ﬁlms can be improved by electro-annealing which is a process of self-heating by electric current [12e14]. Electro-annealing offers many advantages, i.e. no external heater is required during annealing and the direct Joule heat generated by applying an electric ﬁeld to the ﬁlm leads to a decrement in both impurity generation and heat overloading by the surrounding components . Moreover, electro-annealing is suitable for thermally sensitive substrates, because, in the case of electro-annealing, crystallization starts and proceeds faster at lower power levels in contrast to thermal annealing due to efﬁcient energy coupling from Joule heating. Developing a clear under-standing about the characteristics of ITO thinﬁlms under electrical current ﬂow is crucial to eliminate the life-time effects of the electronic devices. However, there is limited research concerned with the investigation of the inﬂuence of electro-annealing on the properties of the ITO thinﬁlms by passing electric currents through them in air and vacuum[12e14]. In the previous studies, Rogozin et al.proposed a method which provides constant power at
* Corresponding author. Department of Physics, Izmir Institute of Technology, 35430, Urla, Izmir, Turkey.
E-mail address:email@example.com(H. Koseoglu).
Contents lists available atScienceDirect
j o u r n a l h o m e p a g e : w w w . e l s e v i e r . c o m / l o c a t e / v a c u u m
http://dx.doi.org/10.1016/j.vacuum.2015.06.027 0042-207X/© 2015 Elsevier Ltd. All rights reserved.
scale applications. 2. Experimental
A large area magnetron sputtering coating system was used for the deposition of the ITO thinﬁlms. The schematic represen-tation of the large area magnetron sputtering coating system can be seen inFig. 1. In this system, the movable sample holder is slowly moved underneath the target via a feedthrough system and theﬁlm thickness depends on the applied power and angular velocity of the feedthrough mechanism. 3 mm thick and 50 mm 60 mm width and length borosilicate glasses were used as substrates. They were cleaned in an ultrasonic bath in the order of acetone, alcohol and de-ionized water for 10 min in each and then theﬁnal cleaning was done by plasma etching for 10 min to remove organic residue. After cleaning the substrates, they were placed onto the sample holder (50 90 cm2). To evacuate the system to below 3.33 106mbar,
we used a rough pump backing a turbo-molecular pump. After evacuation of the chamber 26 sccm Ar and 1 sccm O2gases were
admitted using a massﬂow controller, to maintain the working gas pressure at about 5.6 103mbar. Then, 350 W DC power (ADL Maris, 10 kW) was applied to generate the plasma on the 50 20 cm2ITO target (purity of 99.99% and a weight per cent of
10e90 for SnO2and In2O3). During the ITO thinﬁlm deposition, we
moved the sample holder at 3.0 cm/min, and ITO thinﬁlms with the thickness of 256 nm were grown at 250C substrate temperature which was measured by a thermocouple on the sample holder.
The schematic representation of the electro-annealing process on the ITO thinﬁlms can be seen inFig. 2. 1
mm thick, 5 mm wide and 60 mm length of copper plates were attached to the two opposite edges of the substrates in order to apply a constant cur-rent. After the deposition of the ITO thinﬁlms onto the borosilicate
glasses, electro-annealing was performed by applying 0.75, 1.00, 1.25 and 1.50 A constant ac currents to the ITO thinﬁlms in vacuum (<6.6 106mbar) and air for 10 min. The ITO thinﬁlm temper-ature increased during electro-annealing for 10 min and then naturally decreased to the room temperature within between 20 and 40 min after annealing currents were switched off.
The structural properties of the ITO thinﬁlms were character-ized by an X-ray diffractometer (XRD) (Philips X'Pert Pro) with CuK
l¼ 0.154 nm). The optical properties of the ITO thin ﬁlms were measured by a spectrophotometer (PerkinElmer Lambda 950 UV/Vis/NIR Spectrophotometer) in the 200e2600 nm wavelength range. The sheet resistances (Rs) of ITO thinﬁlms were
measured by the four point probe method using a Keithley 2425 instrument.
3. Results and discussion
Due to the Joule heating, the temperature of the ITO thinﬁlms increases as the electrical current passes through the ﬁlms. The variation of the temperature versus time of electro-annealed thin ﬁlms in air and vacuum are shown inFig. 3. Sample temperature increased during 10 min and then slowly decreased to the room temperature within 20 and 40 min. The highest temperatures for the electro-annealed ITO thinﬁlms at the end of the 10 min in air and vacuum were about 98, 124, 229, 327C and 160, 218, 292, 319C when currents were 0.75, 1.00, 1.25, 1.50 A, respectively. Due to the heat balance between heat input and heat loss, the tem-perature of the ﬁlms during electro-annealing in vacuum was higher as compared to electro-annealing in air for the same current input. In our set up, heat input, radiation and conductance terms of heat loss were approximately the same for electro-annealing in
vacuum and in air. However, only the convection term of heat loss was noticeably higher for electro-annealing in air, and this loss caused lower temperature of theﬁlms during electro-annealing in air.
Sheet resistances (Rs) of the as-grown and electro-annealed ITO
ﬁlms in air and vacuum are shown inFig. 4. The sheet resistances of the ITO thinﬁlms are strongly related to the amount of oxygen vacancies and microstructure . The oxygen vacancies create maximum two free electrons per vacancy to the donor level through ionization, leading to an increase in conductivity. For the electro-annealing in vacuum, the Rsof theﬁlms decreased with
increasing current due to an increase of the temperature by electro-annealing. The decrease in Rscan be attributed to the improvement
in the crystallinity and enhancement of oxygen vacancies which results from releasing of some oxygen atoms from the surface of the ITO thinﬁlms and the absence of free oxygen in vacuum. In com-parison with the electro-annealed ITOﬁlms in vacuum, the sheet resistances of the electro-annealed ITOﬁlms in air are higher due to the reaction of free oxygen in ambient with the ITOﬁlms and less crystallization. For the electro-annealing in air, the Rsof theﬁlms
decreased up to 1.00 A since the lower temperature of theﬁlm
increases the interaction of oxygen atoms with In atoms and the In2O3-xphase is formed. This formation results in the
intensi-ﬁcation of the oxygen vacancy concentration and decrease of the Rs.
For the higher current values, high temperature results in interac-tion of the residual oxygen atoms inside theﬁlm or on the top surface with In atoms and with the In2O3-xphase, after that In2O3
phase is formed. This formation reduces oxygen vacancy concen-tration and increases Rs.
X-ray diffraction (XRD) was used to analyze the effect of electro-annealing on the crystal structure of the ITO thinﬁlms.Fig. 5shows XRD patterns of the as-grown (deposited at 250C) and ITO thin ﬁlms electro-annealed at 0.75, 1.00, 1.25 and 1.50 A in air and vacuum. It should be noted that the broad hump between 20 and 30 (2
q), which occurs due to background from the borosilicate glass substrate, was extracted from the XRD graphs. The XRD pat-terns, which consist of (211), (222), (400), (411), (431), (440) and (622) peaks, of theﬁlms indicate a cubic In2O3phase. None of the
spectra revealed any characteristic peaks of Sn, SnO, or SnO2due to
complete miscibility of tin atoms into the In2O3 lattice. It was
observed that all of the ITO thin ﬁlms are crystalline and have strong (222) and (400) peaks showing preferred orientations. Appearance of the strong (222) and (400) peaks indicates the coexistence of<100> and <111> textures. For all of the electro-annealed ITO thinﬁlms, it can be clearly seen that the crystal-linity of the ﬁlms improves by increasing the electro-annealing current. Moreover, crystalline structures become more perfect for the ITO thinﬁlms electro-annealed in vacuum. This improvement can be clearly seen inFig. 6which shows (222) and (400) reﬂections in detail for the sample electro-annealed in vacuum and in air at 1.5 A. The (222) preferred plane is a close-packed plane in the In2O3
body-centered cubic structure and does not accommodate va-cancies very well. Unlike the (222) preferred plane, the (400) plane accommodates the oxygen vacancies on its planes. Therefore, the sheet resistances of the ITOﬁlms depend upon the orientation of the (400) plane rather than that of (222) plane. As seen inFigs. 5 and 6and , ITO thinﬁlms electro-annealed in vacuum are more oriented along the (400) plane at the same current. This orientation also explains why the sheet resistances of the ITO thinﬁlms electro-annealed in vacuum are lower than those electro-electro-annealed in air.
Fig. 7shows the transmittance spectra as a function of wave-length in the range of 200e2600 nm for the as-grown and the electro-annealed ITO thin ﬁlms at different currents in air and vacuum, respectively. It clearly shows that the electro-annealing process enhances the transmittance ofﬁlms in the visible region. In the visible light region, the average transmittance between
Fig. 3. The variation of temperature versus time of electro-annealed ITO thinﬁlms in a) air and b) vacuum.
Fig. 4. Sheet resistances of electro-annealed ITO thinﬁlms in air and vacuum with applied currents.
400 nm and 800 nm (including borosilicate glass substrate) is about 71% for the as-grown ITO thinﬁlms and it increases up to 82% both for electro-annealing in vacuum and air (Table 1). Moreover, average transmittance increases by increasing current values. Such an increase implies that the optical properties of theﬁlms improve due to the improvement of structural homogeneity of theﬁlms and the decrease of light reﬂection. In the near infrared region, the concentration of free carriers becomes important for the optical transmittance of the ITOﬁlms. FromFig. 4, we observed that there exists a correlation between the NIR transmittance and Rsof
theﬁlms for both electro-annealing in air and vacuum. Lower re-sistivity values result from higher concentration of free carriers that cause higher reﬂection or lower transmission of the infrared region. In the present study, the absorption coefﬁcient,
Fig. 5. XRD patterns of the as grown ITO thinﬁlms and electro-annealed ITO thin ﬁlms in a) air and b) vacuum.
Fig. 6. Detail view of (222) and (400) reﬂections for the sample electro-annealed in vacuum and air at 1.5 A.
Fig. 7. Transmittance spectra as a function of wavelength in the range of 200e2600 nm for the as grown and electro-annealed ITO ﬁlms in a) air and b) vacuum. Table 1
Transmission, sheet resistance and energy gap results of the electro-annealed ITO thinﬁlms in air and vacuum.
I (A) Transmission (%) Rs(U/,) Eg(eV)
Air Vacuum Air Vacuum Air Vacuum 0.00 73.497 73.497 16.761 16.761 4.280 (±0.027) 4.280 (±0.027) 0.75 79.471 79.355 15.402 13.590 4.288 (±0.019) 4.293 (±0.018) 1.00 79.976 80.486 15.266 11.778 4.293 (±0.023) 4.333 (±0.015) 1.25 83.350 82.931 24.190 09.830 4.262 (±0.021) 4.351 (±0.031) 1.50 82.744 82.799 26.319 09.060 4.235 (±0.022) 4.373 (±0.013)
photon energy (h
n) plot was used to estimate the band-gap energy of the ITO thinﬁlms (Fig. 8). Absorption was calculated using the following equation[17,18].
T R ¼ eat (1)
where T and R denote the transmittance and reﬂectance, respec-tively, and t is the thickness of theﬁlm. The reﬂectance of the ﬁlms was neglected due to its relatively low value[17,19], and then the absorption coefﬁcient was simpliﬁed as
Since indium oxide has a direct transition, i.e.
the band-gaps of theﬁlms are deduced from the extrapolation of the linear plots of
The direct optical band-gap values of the electro annealed ITO thinﬁlms in air and vacuum can be seen inTable 1. The electronic gap values obtained from theﬁt of the curves is slightly higher for the samples annealed in vacuum compared to the samples annealed in air for the same current input. This difference may be due to the higher carrier concentrations in the samples electro-annealed in vacuum. We observed that there is a correlation be-tween the band-gap and Rs for all of the electro-annealed thin
ﬁlms, i.e. while the resistivity decreases, the band-gap increases with respect to the increased annealing current. The increase in the band-gap may be due to an increase in the carrier concentrations. This band-gap widening can be explained on the basis of the Bur-steineMoss shift. However, at very high carrier concentrations, there may be band-gap narrowing due to the electroneelectron and electron-impurity scattering.
Understanding the effect of electric current on ITO thin films is essential to increase the life-time of electronic devices. In this study, we analyzed the effect of electro-annealing in air and vac-uum on the structural, optical and electrical properties of the crystalline ITO thin ﬁlms grown by large area DC magnetron sputtering at 250 C substrate temperature. Both for electro-annealing in air and vacuum, we observed improvement in the structural, optical and electrical properties of the ITO thinﬁlms due to the annealing process. In comparison with electro-annealed ITO thinﬁlms in vacuum, higher sheet resistances were
obtained for the electro-annealed ITO thinﬁlms in air. Moreover, for the ITO thinﬁlms electro-annealed in vacuum, the crystallinity of the thinﬁlms was more improved compared to the thin ﬁlms electro-annealed in air. The average transmittances of theﬁlms were increased up to 82% including the borosilicate glass substrate for both electro-annealing in air and vacuum. Ourﬁndings indicate that electro-annealing in vacuum is a more appropriate technique for the applications in the industry.
Dr. Basak Bengu is gratefully acknowledged for supplying bo-rosilicate glass and the authors would like to acknowledge the fa-cilities of Applied Quantum Research Center (AQuReC) for the current study.
 C.W. Tang, S.A. Vanslyke, Organic electroluminescent diodes, Appl. Phys. Lett. 51 (1987) 913.
 G. Li, C.W. Chu, V. Shrotriya, J. Huang, Y. Yang, Efﬁcient inverted polymer solar cells, Appl. Phys. Lett. 88 (2006) 253503.
 L. Zhao, Z. Zhou, H. Peng, R. Cui, Indium tin oxide thinﬁlms by bias magnetron rf sputtering for heterojunction solar cells application, Appl. Surf. Sci. 252 (2005) 385.
 H.M. Kim, K. Bae, S. Sohn, Electronic and optical properties of indium zinc oxide thinﬁlms prepared by using nanopowder target, Jpn. J. Appl. Phys. 50 (2011) 45801.
 D. Barreca, C. Massignan, S. Daolio, M. Fabrizio, C. Piccirillo, L. Armelao, E. Tondello, Composition and microstructure of cobalt oxide thinﬁlms ob-tained from a novel cobalt(II) precursor by chemical vapor deposition, Chem. Mater. 13 (2001) 588.
 K. Ichihara, N. Inoue, M. Okubo, N. Yasuda, The origin of the inhomogeneity of electrical resistivity in magnetron-sputtered indium tin oxide thinﬁlms, Thin Solid Films 245 (1994) 152.
 T. Seikeb, J. Nagai, Electrochromism of 3d transition metal oxides, Sol. Energy Mater. 22 (1991) 107.
 M. Ando, T. Kobayashi, S. Iijima, M. Harita, Optical recognition of CO and H2by
use of gas-sensitive AueCo3O4compositeﬁlms, J. Mater. Chem. 7 (1997) 1779.
 M. Tanaka, M. Mukaia, Y. Fujimuri, M. Kondoh, Y. Tasaka, H. Baba, S. Usami, Transition metal oxideﬁlms prepared by pulsed laser deposition for atomic beam detection, Thin Solid Films 281 (1996) 453.
 O. Tuna, Y. Selamet, G. Aygun, L. Ozyuzer, High quality ITO thinﬁlms grown by DC and RF sputtering without oxygen, J. Phys. D: Appl. Phys. 43 (2010) 055402.
 L. Kerkache, A. Layadi, E. Dogheche, D. Remiens, Physical properties of RF sputtered ITO thinﬁlms and annealing effect, J. Phys. D: Appl. Phys. 39 (2006) 184.
 A. Rogozin, N. Shevchenko, M. Vinnichenko, M. Seidel, A. Kolitsch, W. M€oller, Annealing of indium tin oxide ﬁlms by electric current: properties and structure evolution, Appl. Phys. Lett. 89 (2006) 061908.
 Y. Pei, L. Lin, W. Zheng, Y. Qu, Z. Huang, F. Lai, Effect of passing electric current on the electrical and optical properties of ITOﬁlms in air, Surf. Rev. Lett. 16 Fig. 8.a2versus Photon Energy (hn) curve for the as-grown and electro-annealed ITOﬁlms in a) air and b) vacuum.